Research Inventy: International Journal Of Engineering And ScienceVol.2, Issue 10 (April 2013), Pp 23-27Issn(e): 2278-4721, Issn(p):2319-6483, Www.Researchinventy.Com23Performance Evaluations of Calcium Nitrite on Steel RebarCorrosion in Quarry Dust ConcreteDr.M.Devi,Department of Civil Engineering,Paavai Engineering College, Namakkal-637018, Tamilnadu, India.Abstract: The utilization of quarry dust as fine aggregate in concrete is advantageous because of the benefitssuch as reduction in demand for river sand, environment load and cost of concrete. In this study, experimentalinvestigation has been done to explore the significance of quarry dust as fine aggregate in concrete. Corrosionis the major durability problem causing deterioration of concrete structures. Hence, the objective of this work isto study the strength and corrosion resisting properties of concrete containing quarry dust as fine aggregatealong with calcium nitrite as corrosion inhibiting admixture at the dosage of 1%, 2%, 3% and 4% by weight ofcement. Strength tests, water absorption test and the durability tests were carried out and the results werecompared with the natural sand concrete. The corrosion resistance performance was determined by impressedvoltage method, rapid chloride permeability test and gravimetric weight loss method. The results proved thatquarry dust as substitute for river sand in concrete increases the strength of the concrete, with addition ofinhibitor it proffer very good resistance against corrosion.Key Words: Concrete, quarry dust, super plasticizer, inhibitor, chloride ingress, corrosion resistance,durabilityI. INTRODUCTIONUtilization of quarry dust as fine aggregate in concrete is giving good strength and density and hencelower permeability which enable it to provide better resistance to freeze/thaw cycles and chemical attack inadverse environment [1,2]. A complete replacement of sand by quarry dust in concrete is possible with propergradation of quarry dust before utilization [3,4]. The compressive strength of quarry dust concrete can beimproved with admixture E  and super plasticizers can be used to improve the workability of quarry dustreplaced concrete . Concrete produced using quarry fines shows improvement in higher flexural strength,abrasion resistance, and unit weight which are very important for reducing corrosion or leaching [7,8]. Self-compacting concrete can also be produced using quarry dust . Durability of concrete may be defined as theability of concrete to resist weathering action, chemical attack and abrasion while maintaining its desiredengineering properties [9,10]. Corrosion of reinforcing steel is a major problem facing the concreteinfrastructures [11,12]. Many structures in adverse environments have experienced unacceptable loss inserviceability of safety earlier than anticipated due to the corrosion of reinforcing steel  and thus needreplacement, rehabilitation or strengthening. Corrosion can be prevented by chemical method by using certaincorrosion inhibiting chemical and coating to reinforcement. According to NACE [National Association ofCorrosion Engineers] inhibitors are substances which when added to an environment; decrease the rate of attackon a metal . Corrosion inhibitors function by reinforcing a passive layer or by forming oxide layer andprevent outside agents and reduce the corrosion current [16-18]. Corrosion inhibitors are becoming an acceptedmethod of improving durability of reinforced concrete in chloride laden environments [19,20].This paper dealswith the experimental study to investigate the effect of calcium nitrite as inhibitor in concrete containing quarrydust as fine aggregate in resisting corrosion.II. MATERIALSOrdinary Portland Cement [43 grade] has been used throughout the investigation. River sand,confirmed to grading zone – II as per table 4 of IS 383-1970 has been used as fine aggregate for controlspecimen with specific gravity 2.57, fineness modulus 2.67 and bulk density 1460kg/m3.Quarry dust conformingto grading Zone - II was used as fine aggregate instead of river sand with specific gravity 2.68, fineness modulus2.7 and bulk density 1790kg/m3. Aggregate obtained from nearby granite quarry has been used for this study.The maximum size of aggregate is 20 mm with specific gravity 2.7, and fineness modulus 4.33. Potable tapwater available in the laboratory was used for mixing and curing of concrete. High yield strength deformed barsof diameter 16mm was used for pullout and corrosion tests. To increase the workability of quarry dust concrete
Performance Evaluations Of Calcium Nitrite On Steel…24commercially available super plasticizer ROFF 320 has been used. To attain strength of 20N/mm2a mixtureproportion was designed based on IS: 10262 – 1982 and SP 23: 1982. The mixture was 1: 1.517: 3.38 withwater cement ratio 0.45.III. METHODOLOGYConcrete cubes of size 150 X 150 X 150mm, beams of size 500 X 100 X 100 mm cylinders of size150mm diameter and 300 mm long were cast with and without calcium nitrite for compressive, flexural and splittensile strength. After 24 hours the specimens were demoulded and subjected to water curing. After 3, 7and 28days the specimens were tested as per IS: 516 – 1964. Water absorption of hardened concrete specimens wascalculated based on ASTM C642-81.To assess the corrosion protection efficiency under impressed voltagemethod and weight loss method, concrete cylinders of size 75mm diameter and 150mm length, with centrallyplaced steel rod of 16mm diameter were cast. The steel rod is placed in such a way that a constant cover ismaintained all round. Concrete discs of 100mm diameter and 50mm depth were cast for rapid chloridepermeability test.3.1 Specimen identificationThe various specimen cast are shown in table 1.Table1–Specimen identificationIV. RESULTS AND DISCUSSION4.1 Discussion on conventional concrete and quarry dust replaced concrete:The compressive, split tensile, and flexural strength results after 28 days curing are given in Table 2and figures 1to 3.. When comparing the results of conventional concrete [C ] and quarry dust concrete [Q ], it isobvious that quarry dust replaced concrete specimens have shown improvement in the above strength properties.There was 8.75% increase in compressive strength, 2.5% increase in split tensile strength and 1.68% increase inflexural strength. From the impressed voltage test results it is evident that, the corrosion resistance performanceof quarry dust concrete was 10.62% greater than the conventional concrete. Weight loss measurement result showsthat the corrosion rate of quarry dust concrete specimen decreased by 9.12% when compared with conventionalconcrete. The rapid chloride permeability test results clearly indicate that, the corrosion resistance performanceof quarry dust concrete is 8.84% greater than conventional concrete.Fig . 1Compressive strengthMix DefinitionC Conventional concrete with river sand as fine aggregateQ Quarry dust concrete having quarry dust as fine aggregateQ1 Quarry dust concrete with addition of 1% calcium nitriteQ 2 Quarry dust concrete with addition of 2 % calcium nitriteQ 3 Quarry dust concrete with addition of 3 % calcium nitriteQ 4Quarry dust concrete with addition of 4 % calciumnitrite
Performance Evaluations Of Calcium Nitrite On Steel…25Fig. 2 Split Tensile StrengthFig. 3 Flexural strength Fig.4 Water absorption Test4.2 Discussion on quarry dust concrete with and without inhibitorThe strength test results for concrete containing quarry dust as fine aggregate along with calcium nitriteat 1%, 2%, 3% and 4% are shown in figures 1,2 and 3. The compressive strength results after 28 days curing areshown in figure 1. From the figure it is evident that 1% addition of calcium nitrite shows 3.29% increase in thecompressive strength, while the addition of 2% of this inhibitor gives hike of 7.28% and this yields themaximum increase in the strength value. Further, addition of calcium nitrite to 3% gives 1.64% increase incompressive strength. From fig 2it is observed that quarry dust concrete specimens along with 2% inhibitorshowed the maximum increase in split tensile strength by 5.26 %. However the strength is reducing graduallyfor 3% and 4% addition of inhibitor. All quarry dust replaced specimens with addition of inhibitor have shownslight increase in flexural strength when compared to control specimen Q[fig 3]. Especially the addition of 2%of the inhibitor shows the maximum improvement of 3.53%, %. Among all the percentages 2% Addition ofCalcium nitrite shows maximum improvement in all the strength values. For 3% and 4% addition of inhibitorthere was a slight reduction in strength due to retardation of C3S hydration. Over dosing of corrosion inhibitorsresulted in acceleration in setting time which lead to a reduction in ultimate strength of concrete. In accordancewith figure 4, the water absorption of quarry dust replaced concrete after saturation is found to be less whencompared with ordinary concrete specimens. Among all the percentages of inhibitors added 2% of calciumnitrite was found to be the optimum.V. IMPRESSED VOLTAGE TESTThe specimens were tested by impressed voltage technique and the time taken for initiation ofcorrosion in the specimen is shown in figure 5. Test results have shown that the ordinary concrete specimen Cstarted to corrode after 146 hrs. Specimen with 100% replacement of river sand with quarry dust Q, started at160 hrs. Quarry dust replaced concrete specimen with addition of 1% inhibitor MIX Q1 started after 280hrs. Thespecimen with 2% inhibitor MIX Q2, started after 288 hrs and MIX Q3 with 3% of inhibitor, started to corrodeafter 270 hours and for 4% it was 238 hrs. The above results clearly indicated that corrosion resistance increasedwith increase of percentage of corrosion inhibitor.
Performance Evaluations Of Calcium Nitrite On Steel…26Fig.5 Corrosion initiation timeRapid Chloride Permeability and Weight loss measurementsFig 6 Rapid Chloride Permeability TestFig 7 Corrosion rate with addition of inhibitorFigure 6 shows the chloride diffusion results of the different percentages of inhibitors. The RCPT value forconventional concrete at 28 days is 2678 Coulombs whereas for quarry dust concrete it is found to be 2426Coulombs. The performance of the quarry dust concrete with 1%, 2%, 3% and 4% addition of calcium nitrite areobserved to be 61.9%, 97.87%, 51.05% and 19.27% greater than the control specimen. From the figure it isobserved that addition of 2% calcium nitrite shows lower coulomb values than the other mixes. Corrosion ratefrom the weight – loss measurements [figure 7] clearly indicates that the rate of corrosion decreases with theincrease of percentage of inhibitor up to 2% and further addition shows a slight increase when compared to MIX
Performance Evaluations Of Calcium Nitrite On Steel…27VI. CONCLUSIONFrom the experimental studies the following conclusions were drawn Concrete containing quarry dust as fine aggregate along with appropriate dosage of super plasticizer givesslightly higher strength when compared with conventional concrete Among all the percentages of calcium nitrite added, 2% addition of calcium nitrite shows maximumimprovement in the compressive strength, split tensile strength, and flexural strength when compared to thecontrol specimen. Incorporation of inhibitor decreases permeability & water absorption of quarry dust concrete. The results of corrosion tests indicate that, corrosion initiation time of steel rod embedded quarry dustconcrete is delayed due to the addition of inhibitor and also there was a reduction in corrosion rate. Amongall the percentages of inhibitors 2% was found to be the optimum percentage for getting maximumcorrosion resistance Considering strength as well as durability criteria quarry dust concrete along with 2% of calcium nitrite canbe effectively used in reinforced concrete structures for delaying corrosion and to increase other strengthand durability characteristics.REFERENCES R. Ilangovan And K.Nagamani “Application Of Quarry Rock Dust As Fine Aggregate In Concrete Construction”. NationalJournal On Construction Management: Nicmr, Pune, December.Pp.5-13, 2006 Raman, S.N., Md Safiuddin And Zain, M.F.M. “Non – Destructive Of Flowing Concretes Incorporating Quarry Waste”, AsianJournal Of Civil Engineering [Building And Housing] Vol.8, No.6, Pp. 597 -614,2007. R. Ilangovan, N.Mahendran And K.Nagamani “Strength And Durability Properties Of Concrete Containing Quarry Rock DustAs Fine Aggregate”. Arpn Journal Of Engineering And Applied Science, Vol.3, No.5, October 2008 M.Shahul Hameed And A.S.S.Sekar, “Properties If Green Concrete Containing Quarry Rock Dust And Marble Sludge PowderAs Fine Aggregate” Arpn Journal Of Engineering And Applied Science, Vol.4, No.4, October 2009. R.Murugesan, N.R.Chitra, P.Saravanakumar, “Effect Of Partial Replacement Of Sand By Quarry Dust In Concrete With AndWithout Super Plasticizer” Proceedings Of The National Conference On Concrete Technology For The Future, Pp,167-170,2006. Prachoom Khamput “ A Study Of Compressive Strength Of Concrete Using Quarry Dust As Fine Aggregate And Mixing WithAdmixture Type E”, Rajamangla University Of Technology Thanyaburi, Pathumthani, Thailand, 2005. Sahu A.K., Sunil Kumar And Sachan A.K. “Quarry Stone Waste As Fine Aggregate For Concrete”. The Indian Concrete Journal.Pp. 845-848, 2003. R. Ilangovan And K.Nagamani “Studies On Strength And Behavior Of Concrete By Using Quarry Dust As Fine Aggregate”. CeAnd Cr Journal, Newdelhi. October.Pp.40-42, 2006 . R.Vedalakshmi And N.S.Rengasamy, “Quality Assurance Tests For Corrosion Resistance Of Steel Reinforcement”The IndianConcrete Journal, April 2000. Allan Crane, P. “Corrosion Of Reinforcement In Concrete Construction”, Society Of Chemical Industry, London. PublishersEllis Horwood Ltd., First Edition, 1983. Ha-Won Song, Velu Saraswathy, “ Corrosion Monitoring Of Reinforced Concrete Structures – A Review”, InternationalJournal Of Electrochemical Science, No. 2 , 1- 28 ,2007. Videm, “Corrosion Of Reinforcement In Concrete. Monitoring, Prevention And Rehabilitation”. Efc No: 25. London, Pa.104-121.E, 1998. V.S.Ramachandran, “Concrete Admixtures Handbook” Institute For Research In Construction, National Research CouncilCanada, Ottawa, Ontario, Canada, 2002. Fontana Mars, G. “Corrosion Engineering”, Mcgraw-Hill International Editions, Materials Science And Engineering Series,Singapore,1987. J.Prabakar, P.Devadas Manoharan And M.Neeklamegam, “Performance Evaluation Of Concrete Containing Sodium NitrateInhibitor ” Proceedings Of The 11thInternational Conference On Non-Conventional Materials And Technologies 6-9 September2009, Bath, Uk Berke, N.S.. Hicks, M.C. Predicting Long-Term Durability Of Steel Reinforced Concrete With Calcium Nitrite CorrosionInhibitor. Cement & Concrete Composites 26 191–198, 2004 . Hope,B.B. And Ip, A.K.C “Corrosion Inhibitors For Use In Concrete” Aci Material Journal, V.86.No.3,1989, Pp.602-608,1989. Violetta F. Munteanu And Frederick D.Kinney,"Corrosion Inhibition Properties Of A Complex Inhibitor - Mechanism OfInhibition", Canmet 2000, Pp 255- 269, 2000. De. Schutterg.Luol “Effect Of Corrosion Inhibiting Admixtures On Concrete Properties”Construction And BuildingMaterials,Pp.483-489, 2004. Michael C.Brown, Richard E.Weyers, And Michael M.Sprinkel. “Effect Of Corrosion – Inhibiting Admixtures On MaterialProperties Of Concrete”. Aci Material Journal, V.98. No.3, May- June 2001.